Library of Congress Cataloging-in-Publication DataSmart, Lesley. Solid state chemistry: an introduction/Lesley Smart and Elaine Moore.–3rd ed. p. cm. Includes bibliographical references and index. ISBN 0-7487-7516-1 (alk. paper) 1. Solid state chemistry. I. Moore, Elaine (Elaine A.) II. Title. QD478.S53 2005 541′.0421–dc22 2004058533 Taylor & Francis Group is the Academic Division of T&F Informa plc. Visit the Taylor & Francis Web site at http://www.taylorandfrancis.com and the CRC Press Web site at http://www.crcpress.com
Preface to the Third EditionSolid state and materials chemistry is a rapidly moving field, and the aim of this editionhas been to bring the text as up to date as possible with new developments. A fewchanges of emphasis have been made along the way. Single crystal X-ray diffraction has now been reduced in Chapter 2 to make way for awider range of the physical techniques used to characterize solids, and the number ofsynthetic techniques has been expanded in Chapter 3. Chapter 5 now contains a sectionon fuel cells and electrochromic materials. In Chapter 6, the section on low-dimensionalsolids has been replaced with sections on conducting organic polymers, organicsuperconductors, and fullerenes. Chapter 7 now covers mesoporous solids and ALPOs,and Chapter 8 includes a section on photonics. Giant magnetoresistance (GMR) andcolossal magnetoresistance (CMR) have been added to Chapter 9, and p-wave (triplet)superconductors to Chapter 10. Chapter 11 is new, and looks at the solid state chemicalaspects of nanoscience. We thank our readers for the positive feedback on first two editions and for the helpfuladvice which has led to this latest version. As ever, we thank our friends in the Chemistry Department at the OU, who have beensuch a pleasure to work with over the years, and have made enterprises such as thispossible.
Preface to the Second EditionWe were very pleased to be asked to prepare a second edition of this book. When wetried to decide on the changes (apart from updating) to be made, the advice from oureditor was “if it ain’t broke, don’t fix it.” However, the results of a survey of our usersrequested about five new subjects but with the provisos that nothing was taken out, thatthe book didn’t get much longer, and, above all, that it didn’t increase in price! Therefore,what you see here is an attempt to do the impossible, and we hope that we have satisfiedsome, if not all, of the requests. The main changes from the first edition are two new chapters: Chapter 2 on X-raydiffraction and Chapter 3 on preparative methods. A short discussion of symmetryelements has been included in Chapter 1. Other additions include an introduction toALPOs and to clay minerals in Chapter 7 and to ferroelectrics in Chapter 9. We decidedthat there simply was not enough room to cover the Phase Rule properly and for that werefer you to the excellent standard physical chemistry texts, such as Atkins. We hope thatthe book now covers most of the basic undergraduate teaching material on solid statechemistry. We are indebted to Professor Tony Cheetham for kindling our interest in this subjectwith his lectures at Oxford University and the beautifully illustrated articles that he andhis collaborators have published over the years. Our thanks are also due to Dr. PaulRaithby for commenting on part of the manuscript. As always, we thank our colleagues at the Open University for all their support andespecially the members of the lunch club, who not only keep us sane, but also keep uslaughing. Finally, thanks go to our families for putting up with us and particularly to ourchildren for coping admirably with two increasingly distracted academic mothers—ourbook is dedicated to them. Lesley E.Smart and Elaine A.Moore Open University, Walton Hall, Milton Keynes
Preface to the First EditionThe idea for this book originated with our involvement in an Open University inorganicchemistry course (S343: Inorganic Chemistry). When the Course Team met to decide thecontents of this course, we felt that solid state chemistry had become an interesting andimportant area that must be included. It was also apparent that this area was playing alarger role in the undergraduate syllabus at many universities, due to the exciting newdevelopments in the field. Despite the growing importance of solid state chemistry, however, we found that therewere few textbooks that tackled solid state theory from a chemist’s rather than aphysicist’s viewpoint. Of those that did most, if not all, were aimed at final yearundergraduates and postgraduates. We felt there was a need for a book written from achemist’s viewpoint that was accessible to undergraduates earlier in their degreeprogramme. This book is an attempt to provide such a text. Because a book of this size could not cover all topics in solid state chemistry, we havechosen to concentrate on structures and bonding in solids, and on the interplay betweencrystal and electronic structure in determining their properties. Examples of solid statedevices are used throughout the book to show how the choice of a particular solid for aparticular device is determined by the properties of that solid. Chapter 1 is an introduction to crystal structures and the ionic model. It introducesmany of the crystal structures that appear in later chapters and discusses the concepts ofionic radii and lattice energies. Ideas such as close-packed structures and tetrahedral andoctahedral holes are covered here; these are used later to explain a number of solid stateproperties. Chapter 2 introduces the band theory of solids. The main approach is via the tightbinding model, seen as an extension of the molecular orbital theory familiar to chemists.Physicists more often develop the band model via the free electron theory, which isincluded here for completeness. This chapter also discusses electronic conductivity insolids and in particular properties and applications of semiconductors. Chapter 3 discusses solids that are not perfect. The types of defect that occur and theway they are organized in solids forms the main subject matter. Defects lead tointeresting and exploitable properties and several examples of this appear in this chapter,including photography and solid state batteries. The remaining chapters each deal with a property or a special class of solid. Chapter 4covers low-dimensional solids, the properties of which are not isotropic. Chapter 5 dealswith zeolites, an interesting class of compounds used extensively in industry (as catalysts,for example), the properties of which strongly reflect their structure. Chapter 6 deals withoptical properties and Chapter 7 with magnetic properties of solids. Finally, Chapter 8explores the exciting field of superconductors, particularly the relatively recentlydiscovered high temperature superconductors. The approach adopted is deliberately nonmathematical, and assumes only the chemicalideas that a first-year undergraduate would have. For example, differential calculus is
used on only one or two pages and non-familiarity with this would not hamper anunderstanding of the rest of the book; topics such as ligand field theory are not assumed. As this book originated with an Open University text, it is only right that we shouldacknowledge the help and support of our colleagues on the Course Team, in particularDr. David Johnson and Dr. Kiki Warr. We are also grateful to Dr. Joan Mason who readand commented on much of the script, and to the anonymous reviewer to whomChapman & Hall sent the original manuscript and who provided very thorough and usefulcomments. The authors have been sustained through the inevitable drudgery of writing by anenthusiasm for this fascinating subject. We hope that some of this transmits itself to thestudent. Lesley E.Smart and Elaine A.Moore OU, Walton Hall, Milton Keynes
About the AuthorsLesley E.Smart studied chemistry at Southampton University. After completing a Ph.D.in Raman spectroscopy, also at Southampton, she moved to a lectureship at the RoyalUniversity of Malta. After returning to the United Kingdom, she took an SRC Fellowshipto Bristol University to work on X-ray crystallography for 3 years. Since 1977, she hasworked at the Open University as a lecturer, and then senior lecturer (2000), in inorganicchemistry. At the Open University, she has been involved in the production ofundergraduate courses in inorganic and physical chemistry. Most recently, she was thecoordinating editor of The Molecular World course, which has been copublished with theRSC as a series of eight books. She was also an author on two of these, The ThirdDimension and Separation, Purification and Identification. Her research interests are in the characterization of the solid state, and she has over 40publications in single-crystal Raman studies, X-ray crystallography, zintl phases,pigments, and heterogeneous catalysis. Solid State Chemistry was first produced in 1992. Since then, it has been translatedinto French, German, Spanish, and Japanese. Elaine A.Moore studied chemistry as an undergraduate at Oxford University and thenstayed on to complete a D.Phil, in theoretical chemistry with Peter Atkins. After a 2-year,postdoctoral position at Southampton, she joined the Open University in 1975 as courseassistant, becoming a lecturer in Chemistry in 1977 and Senior lecturer in 1998. She hasproduced OU teaching texts in chemistry for courses at levels 1, 2, and 3 and has writtentexts in astronomy at level 2. The text Molecular Modelling and Bonding, which formspart of the OU Level 2 Chemistry Course, was copublished by the Royal Society ofChemistry as part of The Molecular World series. She oversaw the introduction ofmultimedia into chemistry courses and designed multimedia material for levels 1 and 2.She is coauthor, with Dr. Rob Janes of the Open University, of Metal-Ligand Bonding,which is part of a level 3 Course in Inorganic Chemistry and copublished with the RoyalSociety of Chemistry. Her research interests are in theoretical chemistry applied to solid state systems and toNMR spectroscopy. She is author or coauthor on over 40 papers in scientific journals.She was coauthor of an article in Chemical Reviews on nitrogen NMR spectroscopy ofmetal nitrosyl complexes.
BASIC SI UNITSPhysical quantity (and symbol) Name of SI unit Symbol for unitLength (l) Metre mMass (m) Kilogram kgTime (t) Second sElectric current (I) Ampere AThermodynamic temperature (T) Kelvin KAmount of substance (n) Mole molLuminous intensity (Iv) Candela cdDERIVED SI UNITSPhysical quantity (and Name of SI Symbol for SI derived unit andsymbol) unit definition of unitFrequency (v) Hertz Hz (=s−1)Energy (U), enthalpy (H) Joule J (=kg m2 s−2)Force Newton N (=kg m s−2=J m−1)Power Watt W (=kg m2 s−3=J s−1)Pressure (p) Pascal Pa (=kg m−1 s−2=N m−2=J m−3)Electric charge (Q) Coulomb C (=A s)Electric potential difference (V) Volt V(=kg m2 s−3 A−1=J A−1 s−1)Capacitance (c) Farad F (=A2 s4 kg−1 m−2=A s V−1= A2 s2 J−1)Resistance (R) Ohm Ω (=V A−1)Conductance (G) Siemen S (=A V−1)Magnetic flux density (B) Tesla T (=V s m−2=J C−1 s m−2)SI PREFIXES10–18 10–15 10–12 10–9 10–6 10–3 10–2 10–1 103 106 109 1012 1015 1018 alto femto pico nano micro milli centi deci kilo mega giga tera peta exa a f p n µ m c d k M G T P EFUNDAMENTAL CONSTANTSConstant Symbol ValueSpeed of light in a vacuum c 2.997925×108 m s−1
Charge of a proton e 1.602189×10–19 CCharge of an electron −eAvogadro constant NA 6.022045×1023 mol−1Boltzmann constant k 1.380662×10–23 J K−1Gas constant R=NAk 8.31441 J K−1 mol−1Faraday constant F=NAe 9.648456×104 mol−1Planck constant h 6.626176×10–34 J s 1.05457×10–34 J sVacuum permittivity ε0 8.854×10–12 F m−1Vacuum permeability µ0 4π×10–7 J s2 C−2 m−1Bohr magneton µB 9.27402×10–24 J T−1Electron g value ge 2.00232MISCELLANEOUS PHYSICAL QUANTITIESName of physical quantity Symbol SI unitEnthalpy H JEntropy S J K−1Gibbs function G JStandard change of molar enthalpy J mol−1Standard of molar entropy J K−1 mol−1Standard change of molar Gibbs functionz J mol−1Wave number cm−1Atomic number Z DimensionlessConductivity σ S m−1Molar bond dissociation energy Dm J mol−1Molar mass kg mol−1THE GREEK ALPHABETalpha A α nu N vbeta B β xi Ξ ξ
gamma Γ γ omicron O odelta ∆ δ pi Π πepsilon E ε rho P ρzeta Z ζ sigma ∑ σeta H η tau T τtheta Θ θ upsilon Y υiota I ι phi Φ φkappa K κ chi X χlambda Λ λ psi Ψ ψmu M µ omega Ω ω PERIODIC CLASSIFICATION OF THE ELEMENTS
Table of Contents Chapter 1 An Introduction to Crystal Structures 1 Chapter 2 Physical Methods for Characterizing Solids 91 Chapter 3 Preparative Methods 148 Chapter 4 Bonding in Solids and Electronic Properties 179Chapters 5 Defects and Non-Stoichiometry 201 Chapter 6 Carbon-Based Electronics 282 Chapter 7 Zeolites and Related Structures 301 Chapter 8 Optical Properties of Solids 342 Chapter 9 Magnetic and Dielectric Properties 365Chapter 10 Superconductivity 394Chapter 11 Nanoscience 412 Further Reading 442 Answers Odd Number Questions 446 Index 463
Third EditionSOLID STATE CHEMISTRY An Introduction
1 An Introduction to Crystal StructuresIn the last decade of the twentieth century, research into solid state chemistry expandedvery rapidly, fuelled partly by the dramatic discovery of ‘high temperature’ ceramicoxide superconductors in 1986, and by the search for new and better materials. We haveseen immense strides in the development and understanding of nano-technology, micro-and meso-porous solids, fuel cells, and the giant magnetoresistance effect, to mention buta few areas. It would be impossible to cover all of the recent developments in detail in atext such as this, but we will endeavour to give you a flavour of the excitement that someof the research has engendered, and perhaps more importantly the background withwhich to understand these developments and those which are yet to come. All substances, except helium, if cooled sufficiently form a solid phase; the vastmajority form one or more crystalline phases, where the atoms, molecules, or ions packtogether to form a regular repeating array. This book is concerned mostly with thestructures of metals, ionic solids, and extended covalent structures; structures which donot contain discrete molecules as such, but which comprise extended arrays of atoms orions. We look at the structure and bonding in these solids, how the properties of a soliddepend on its structure, and how the properties can be modified by changes to thestructure. 1.1 INTRODUCTIONTo understand the solid state, we need to have some insight into the structure of simplecrystals and the forces that hold them together, so it is here that we start this book.Crystal structures are usually determined by the technique of X-ray crystallography.This technique relies on the fact that the distances between atoms in crystals are of thesame order of magnitude as the wavelength of X-rays (of the order of 1 Å or 100 pm): acrystal thus acts as a three-dimensional diffraction grating to a beam of X-rays. Theresulting diffraction pattern can be interpreted to give the internal positions of the atomsin the crystal very precisely, thus defining interatomic distances and angles. (Some of theprinciples underlying this technique are discussed in Chapter 2, where we review thephysical methods available for characterizing solids.) Most of the structures discussed inthis book will have been determined in this way. The structures of many inorganic crystal structures can be discussed in terms of thesimple packing of spheres, so we will consider this first, before moving on to the moreformal classification of crystals.
Solid state chemistry 2 1.2 CLOSE-PACKINGThink for the moment of an atom as a small hard sphere. Figure 1.1 shows two possiblearrangements for a layer of such identical atoms. On squeezing the square layer in Figure1.1 (a), the spheres would move to the positions in Figure 1.1 (b) so that the layer takesup less space. The layer in Figure 1.1 (b) (layer A) is called close-packed. To build up aclose-packed structure in three-dimensions we must now add a second layer (layer B).The spheres of the second layer sit in half of the hollows of the first layer: these havebeen marked with dots and crosses. The layer B in Figure 1.2 sits over the hollowsmarked with a cross (although it makes no difference which type we chose). When weadd a third layer, there are two possible positions where it can go. First, it could godirectly over layer A, in the unmarked hollows: if we then repeated this stackingsequence we would build up the layers ABABABA …and so on. This is known ashexagonal close-packing (hcp) (Figure 1.3(a)). In this structure, the hollows markedwith a dot are never occupied by spheres, leaving very small channels through the layers(Figure 1.3(b)). Second, the third layer could be positioned over those hollows marked with a dot. Thisthird layer, which we could label C, would not be directly over either A or B, and thestacking sequence when repeated would be ABC ABC AB…and so on. This is known ascubic close-packing (ccp) (Figure 1.4). (The names hexagonal and cubic for thesestructures arise from the resulting symmetry of the structure—this will be discussed morefully later on.) Close-packing represents the most efficient use of space when packing identicalspheres—the spheres occupy 74% of the volume: the packing efficiency is said to be74%. Each sphere in the structure is surrounded by twelve equidistant neighbours—six inthe same layer, three in the layer above and three in the layer below: the coordinationnumber of an atom in a close-packed structure is thus 12. Another important feature of close-packed structures is the shape and number of thesmall amounts of space trapped in between the spheres. Two different types of space arecontained within a close-packed structure: the first we will consider is called anoctahedral hole. Figure 1.5(a) shows two close-packed layers again but now with theoctahedral holes shaded. Six spheres surround each of these holes: three in layer A andthree in layer B. The centres of these spheres lay at the corners
An introduction to crystal structures 3 FIGURE 1.1 (a) A square array of spheres; (b) a close-packed layer of spheres.
Solid state chemistry 4FIGURE 1.2 Two layers of close-packed spheres.
An introduction to crystal structures 5 FIGURE 1.3 (a) Three hcp layers showing the ABAB…stacking sequence; (b) three hcp layers showing the narrow channels through the layers.of an octahedron, hence the name (Figure 1.5(b)). If n spheres are in the array, then thereare also n octahedral holes. Similarly, Figure 1.6(a) shows two close-packed layers, now with the second type ofspace, tetrahedral holes, shaded. Four spheres surround each of these holes with centresat the corners of a tetrahedron (Figure 1.6(b)). If n spheres are in the array, then there are2n tetrahedral holes. The octahedral holes in a close-packed structure are much bigger than the tetrahedralholes—they are surrounded by six atoms instead of four. It is a matter of simple geometryto calculate that the radius of a sphere that will just fit in an FIGURE 1.4 Three ccp layers.
Solid state chemistry 6 FIGURE 1.5 (a) Two layers of close- packed spheres with the enclosed octahedral holes shaded; (b) a computer representation of an octahedral hole.octahedral hole in a close-packed array of spheres of radius r is 0.414r. For a tetrahedralhole, the radius is 0.225r (Figure 1.7). Of course, innumerable stacking sequences are possible when repeating close-packedlayers; however, the hexagonal close-packed and cubic close-packed are those of
An introduction to crystal structures 7maximum simplicity and are most commonly encountered in the crystal structures of thenoble gases and of the metallic elements. Only two other stacking sequences are found inperfect crystals of the elements: an ABAC repeat in La, Pr, Nd, and Am, and a nine-layerrepeat ABACACBCB in Sm. FIGURE 1.6 (a) Two layers of close- packed spheres with the tetrahedral holes shaded; (b) a computer representation of a tetrahedral hole.
Solid state chemistry 8 FIGURE 1.7 (a) A sphere of radius 0.414r fitting into an octahedral hole; (b) a sphere of radius 0.225r fitting into a tetrahedral hole. 1.3 BODY-CENTRED AND PRIMITIVE STRUCTURESSome metals do not adopt a close-packed structure but have a slightly less efficientpacking method: this is the body-centred cubic structure (bcc), shown in Figure 1.8.(Unlike the previous diagrams, the positions of the atoms are now represented here—andin subsequent diagrams—by small spheres which do not touch: this is merely a device toopen up the structure and allow it to be seen more clearly—the whole question of atomand ion size is discussed in Section 1.6.4.) In this structure an atom in the middle of acube is surrounded by eight identical and equidistant atoms at the corners of the cube—
An introduction to crystal structures 9the coordination number has dropped from twelve to eight and the packing efficiency isnow 68%, compared with 74% for close-packing.The simplest of the cubic structures is the primitive cubic structure. This is built byplacing square layers like the one shown in Figure 1.1 (a), directly on top of one another.Figure 1.9(a) illustrates this, and you can see in Figure 1.9(b) that each atom sits at thecorner of a cube. The coordination number of an atom in this structure is six. Themajority of metals have one of the three basic structures: hcp, ccp, or bcc. Poloniumalone adopts the primitive structure. The distribution of the packing types among themost stable forms of the metals at 298 K is shown in Figure 1.10. As we noted earlier, avery few metals have a mixed hcp/ccp structure of a more complex type. The structuresof the actinides tend to be rather complex and are not included. FIGURE 1.8 Body-centred cubic array.
Solid state chemistry 10FIGURE 1.9 (a) Two layers of aprimitive cubic array; (b) a cube ofatoms from this array.FIGURE 1.10 Occurrence of packingtypes among the metals.
An introduction to crystal structures 11 1.4 SYMMETRYBefore we take the discussion of crystalline structures any further, we will look at thesymmetry displayed by structures. The concept of symmetry is an extremely useful onewhen it comes to describing the shapes of both individual molecules and regularrepeating structures, as it provides a way of describing similar features in differentstructures so that they become unifying features. The symmetry of objects in everydaylife is something that we tend to take for granted and recognize easily without having tothink about it. Take some simple examples illustrated in Figure 1.11. If you imagine amirror dividing the spoon in half along the plane indicated, then you can see that
Solid state chemistry 12 FIGURE 1.11 Common objects displaying symmetry: (a) a spoon, (b) a paintbrush, (c) a snowflake, and (d) a 50p coin.one-half of the spoon is a mirror image or reflection of the other. Similarly, with thepaintbrush, only now two mirror planes at right angles divide it. Objects can also possess rotational symmetry. In Figure 1.11(c) imagine an axlepassing through the centre of the snowflake; in the same way as a wheel rotates about an
An introduction to crystal structures 13axle, if the snowflake is rotated through of a revolution, then the new position isindistinguishable from the old. Similarly, in Figure 1.11(d), rotating the 50p coin by ofa revolution brings us to the same position as we started (ignoring the pattern on thesurface). The symmetry possessed by a single object that describes the repetition ofidentical parts of the object is known as its point symmetry. Actions such as rotating a molecule are called symmetry operations, and therotational axes and mirror planes possessed by objects are examples of symmetryelements. Two forms of symmetry notation are commonly used. As chemists, you will comeacross both. The Schoenflies notation is useful for describing the point symmetry ofindividual molecules and is used by spectroscopists. The Hermann-Mauguin notationcan be used to describe the point symmetry of individual molecules but in addition canalso describe the relationship of different molecules to one another in space—their so-called space-symmetry—and so is the form most commonly met in crystallography andthe solid state. We give here the Schoenflies notation in parentheses after the Hermann-Mauguin notation. 1.4.1 AXES OF SYMMETRYAs discussed previously for the snowflake and the 50p coin, molecules and crystals canalso possess rotational symmetry. Figure 1.12 illustrates this for several molecules. In Figure 1.12(a) the rotational axis is shown as a vertical line through the O atom inOF2; rotation about this line by 180° in the direction of the arrow, produces an identicallooking molecule. The line about which the molecule rotates is called an axis ofsymmetry, and in this case, it is a twofold axis because we have to perform the operationtwice to return the molecule to its starting position. Axes of symmetry are denoted by the symbol n (Cn), where n is the order of the axis.Therefore, the rotational axis of the OF2 molecule is 2 (C2). The BF3 molecule in Figure 1.12(b) possesses a threefold axis of symmetry, 3 (C3),because each of a revolution leaves the molecule looking the same, and three turnsbrings the molecule back to its starting position. In the same way, the XeF4 molecule in(c) has a fourfold axis, 4 (C4), and four quarter turns are necessary to bring it back to thebeginning. All linear molecules have an ∞ (C∞) axis, which is illustrated for the BeF2molecule in (d); however small a fraction of a circle it is rotated through, it always looksidentical. The smallest rotation possible is 1/∞, and so the axis is an infinite-order axis ofsymmetry. 1.4.2 PLANES OF SYMMETRYMirror planes occur in isolated molecules and in crystals, such that everything on oneside of the plane is a mirror image of the other. In a structure, such a mirror
Solid state chemistry 14FIGURE 1.12 Axes of symmetry inmolecules: (a) twofold axis in OF2, (b)
An introduction to crystal structures 15 threefold axis in BF3, (c) fourfold axis in XeF4, and (d) ∞-fold axis in BeF2. FIGURE 1.13 Planes of symmetry in molecules: (a) planes of symmetry in OF2, (b) planes of symmetry in BF3, and (c) planes of symmetry in XeF4.plane is known as a plane of symmetry and is given the symbol m (σ). Molecules maypossess one or more planes of symmetry, and the diagrams in Figure 1.13 illustrate someexamples. The planar OF2 molecule has two planes of symmetry (Figure 1.13(a)), one isthe plane of the molecule, and the other is at right angles to this. For all planar molecules,the plane of the molecule is a plane of symmetry. The diagrams for BF3 and XeF4 (alsoplanar molecules) only show the planes of symmetry which are perpendicular to the planeof the molecule. 1.4.3 INVERSIONThe third symmetry operation that we show in this section is called inversion through acentre of symmetry and is given the symbol (i). In this operation you have to imagine aline drawn from any atom in the molecule, through the centre of symmetry and thencontinued for the same distance the other side; if for every atom, this meets with anidentical atom on the other side, then the molecule has a centre of symmetry. Of themolecules in Figure 1.12, XeF4 and BeF2 both have a centre of symmetry, and BF3 andOF2 do not.
Solid state chemistry 16 1.4.4 INVERSION AXES AND IMPROPER SYMMETRY AXESThe final symmetry element is described differently by the two systems, although bothdescriptions use a combination of the symmetry elements described previously. TheHermann-Mauguin inversion axis is a combination of rotation and inversion and is giventhe symbol The symmetry element consists of a rotation by 1/n of a revolution aboutthe axis, followed by inversion through the centre of symmetry. An example of aninversion axis is shown in Figure 1.14 for a tetrahedral molecule such as CF4. Themolecule is shown inside a cube as this makes it easier to see the FIGURE 1.14 The (S4) inversion (improper) axis of symmetry in the tetrahedral CF4 molecule.
An introduction to crystal structures 17symmetry elements. Rotation about the axis through 90° takes F1 to the position shown asa dotted F; inversion through the centre then takes this atom to the F3 position. The equivalent symmetry element in the Schoenflies notation is the improper axis ofsymmetry, Sn, which is a combination of rotation and reflection. The symmetry elementconsists of a rotation by 1/n of a revolution about the axis, followed by reflection througha plane at right angles to the axis. Figure 1.14 thus presents an S4 axis, where the F1rotates to the dotted position and then reflects to F2. The equivalent inversion axes andimproper symmetry axes for the two systems are shown in Table 1.1. 1.4.5 SYMMETRY IN CRYSTALSThe discussion so far has only shown the symmetry elements that belong to individualmolecules. However, in the solid state, we are interested in regular arrays of TABLE 1.1 Equivalent symmetry elements in the Schoenflies and Hermann-Mauguin Systems Schoenflies Hermann-Mauguin S1≡m S2≡i S3 S4 S6atoms, ions, and molecules, and they too are related by these same symmetry elements.Figure 1.15 gives examples (not real) of how molecules could be arranged in a crystal. In(a), two OF2 molecules are related to one another by a plane of symmetry; in (b), threeOF2 molecules are related to one another by a threefold axis of symmetry; in (c), two OF2molecules are related by a centre of inversion. Notice that in both (b) and (c), themolecules are related in space by a symmetry element that they themselves do notpossess, this is said to be their site symmetry.
Solid state chemistry 18 FIGURE 1.15 Symmetry in solids: (a) two OF2 molecules related by a plane of symmetry, (b) three OF2 molecules related by a threefold axis of symmetry, and (c) two OF2 molecules related by a centre of inversion. 1.5 LATTICES AND UNIT CELLSCrystals are regular shaped solid particles with flat shiny faces. It was first noted byRobert Hooke in 1664 that the regularity of their external appearance is a reflection of ahigh degree of internal order. Crystals of the same substance, however, vary in shapeconsiderably. Steno observed in 1671 that this is not because their internal structurevaries but because some faces develop more than others do. The angle between similarfaces on different crystals of the same substance is always identical. The constancy of theinterfacial angles reflects the internal order within the crystals. Each crystal is derivedfrom a basic ‘building block’ that continuously repeats, in all directions, in a perfectlyregular way. This building block is known as the unit cell.
An introduction to crystal structures 19 To talk about and compare the many thousands of crystal structures that are known,there has to be a way of defining and categorizing the structures. This is achieved bydefining the shape and symmetry of each unit cell as well as its size and the positions ofthe atoms within it. 1.5.1 LATTICESThe simplest regular array is a line of evenly spaced objects, such as those depicted bythe commas in Figure 1.16(a). There is a dot at the same place in each object: if we nowremove the objects leaving the dots, we have a line of equally spaced dots, spacing a,(Figure 1.16(b)). The line of dots is called the lattice, and each lattice point (dot) musthave identical surroundings. This is the only example of a one-dimensional lattice and itcan vary only in the spacing a. Five two-dimensional lattices are possible, and examplesof these can be seen every day in wallpapers and tiling. 1.5.2 ONE- AND TWO-DIMENSIONAL UNIT CELLSThe unit cell for the one-dimensional lattice in Figure 1.16(a) lies between the twovertical lines. If we took this unit cell and repeated it over again, we would reproduce theoriginal array. Notice that it does not matter where in the structure we place the FIGURE 1.16 A one-dimensional lattice (a,b) and the choice of unit cells (c).
Solid state chemistry 20 FIGURE 1.17 Choice of unit cell in a square two-dimensional lattice.lattice points as long as they each have identical surroundings. In Figure 1.16(c), we havemoved the lattice points and the unit cell, but repeating this unit cell will still give thesame array—we have simply moved the origin of the unit cell. There is never one uniqueunit cell that is ‘correct.’ Many can always be chosen, and the choice depends both onconvenience and convention. This is equally true in two and three dimensions. The unit cells for the two-dimensional lattices are parallelograms with their corners atequivalent positions in the array (i.e., the corners of a unit cell are lattice points). InFigure 1.17, we show a square array with several different unit cells depicted. All ofthese, if repeated, would reproduce the array: it is conventional to choose the smallest cellthat fully represents the symmetry of the structure. Both unit cells (1a) and (1b) are thesame size but clearly (1a) shows that it is a square array, and this would be theconventional choice. Figure 1.18 demonstrates the same principles but for a centredrectangular array, where (a) would be the conventional choice because it includesinformation on the centring; the smaller unit cell (b) loses this information. It is alwayspossible to define a non-centred oblique unit cell, but doing so may lose informationabout the symmetry of the lattice. Unit cells, such as (1a) and (1b) in Figure 1.17 and (b) in Figure 1.18, have a latticepoint at each corner. However, they each contain one lattice point because four adjacentunit cells share each lattice point. They are known as primitive unit cells and are giventhe symbol P. The unit cell marked (a) in Figure 1.18 contains
An introduction to crystal structures 21 FIGURE 1.18 Choice of unit cell in a centred-rectangular lattice. FIGURE 1.19 An a glide perpendicular to b.two lattice points—one from the shared four corners and one totally enclosed within thecell. This cell is said to be centred and is given the symbol C. 1.5.3 TRANSLATIONS SYMMETRY ELEMENTSSection 1.4 introduced the idea of symmetry, both in individual molecules and forextended arrays of molecules, such as are found in crystals. Before going on to discussthree-dimensional lattices and unit cells, it is important to introduce two more symmetryelements; these elements involve translation and are only found in the solid state. The glide plane combines translation with reflection. Figure 1.19 is an example ofthis symmetry element. The diagram shows part of a repeating three-dimensionalstructure projected on to the plane of the page; the circle represents a molecule or ion inthe structure and there is distance a between identical positions in the structure. The +sign next to the circle indicates that the molecule lies above the plane of the page in the zdirection. The plane of symmetry is in the xz plane perpendicular to the paper, and isindicated by the dashed line. The symmetry element consists of reflection through thisplane of symmetry, followed by translation. In this case, the translation can be either inthe x or in the z direction (or along a diagonal), and the translation distance is half of the
Solid state chemistry 22repeat distance in that direction. In the example illustrated, the translation takes place inthe x direction. The repeat distance between identical molecules is a, and so thetranslation is by a/2, and the symmetry element is called an a glide. You will notice twothings about the molecule generated by this symmetry element: first, it still has a + signagainst it, because the reflection in the plane leaves the z coordinate the same and second,it now has a comma on it. Some molecules when they are reflected through a plane ofsymmetry are enantiomorphic, which means that they are not superimposable on theirmirror image: the presence of the comma indicates that this molecule could be anenantiomorph. The screw axis combines translation with rotation. Screw axes have the generalsymbol ni where n is the rotational order of the axis (i.e., twofold, threefold, etc.), and thetranslation distance is given by the ratio i/n. Figure 1.20 illustrates a 21 screw axis. In thisexample, the screw axis lies along z and so the translation must be in FIGURE 1.20 A 21 screw axis along z.the z direction, by c/2, where c is the repeat distance in the z direction. Notice that in thiscase the molecule starts above the plane of the paper (indicated by the + sign) but theeffect of a twofold rotation is to take it below the plane of the paper (− sign). Figure 1.21probably illustrates this more clearly, and shows the different effects that rotational andscrew axes of the same order have on a repeating structure. Rotational and screw axesproduce objects that are superimposable on the original. All other symmetry elements—glide plane, mirror plane, inversion centre, and inversion axis—produce a mirror imageof the original. 1.5.4 THREE-DIMENSIONAL UNIT CELLSThe unit cell of a three-dimensional lattice is a parallelepiped defined by three distancesa, b, and c, and three angles α, β, and γ, as shown in Figure 1.22. Because the unit cells
An introduction to crystal structures 23are the basic building blocks of the crystals, they must be space-filling (i.e., they mustpack together to fill all space). All the possible unit cell shapes that can fulfill thiscriterion are illustrated in Figure 1.23 and their specifications are listed in Table1.2.These are known as the seven crystal systems or classes.These unit cell shapes aredetermined by minimum symmetry requirements which are also detailed in Table 1.2. The three-dimensional unit cell includes four different types (see Figure 1.24):1. The primitive unit cell—symbol P—has a lattice point at each corner.2. The body-centred unit cell—symbol I—has a lattice point at each corner and one at the centre of the cell.3. The face-centred unit cell—symbol F—has a lattice point at each corner and one in the centre of each face.4. The face-centred unit cell—symbol A, B, or C—has a lattice point at each corner, and one in the centres of one pair of opposite faces (e.g., an A-centred cell has lattice points in the centres of the bc faces). FIGURE 1.21 Comparison of the effects of twofold and threefold rotation axes and screw axes.
Solid state chemistry 24When these four types of lattice are combined with the 7 possible unit cell shapes, 14permissible Bravais lattices (Table 1.3) are produced. (It is not possible to combinesome of the shapes and lattice types and retain the symmetry requirements listed in Table1.2. For instance, it is not possible to have an A-centred, cubic, unit cell; if only two ofthe six faces are centred, the unit cell necessarily loses its cubic symmetry.) FIGURE 1.22 Definition of axes, unit cell dimensions, and angles for a general unit cell.
An introduction to crystal structures 25 FIGURE 1.23 (a) The unit cells of the seven crystal systems, (b) Assemblies of cubic unit cells in one, two, and three dimensions.The symmetry of a crystal is a point group taken from a point at the centre of a perfectcrystal. Only certain point groups are possible because of the constraint made by the factthat unit cells must be able to stack exactly with no spaces—so only one-, two-, three-,
Solid state chemistry 26four-, and sixfold axes are possible. Combining this with planes of symmetry and centresof symmetry, we find 32 point groups that can describe the shapes of perfect crystals. If we combine the 32 crystal point groups with the 14 Bravais lattices we find 230three-dimensional space groups that crystal structures can adopt (i.e., 230 TABLE 1.2 The seven crystal systemsSystem Unit cell Minimum symmetry requirementsTriclinic α≠β≠γ≠90° None a≠b≠cMonoclinic α=γ=90° One twofold axis or one symmetry plane β≠90° a≠b≠cOrthorhombic α=β=γ=90° Any combination of three mutually perpendicular twofold a≠b≠c axes or planes of symmetryTrigonal/rhombohedral α=β=γ≠90° One threefold axis a=b=cHexagonal α=β=90° One sixfold axis or one sixfold improper axis γ=120° a=b≠cTetragonal α=β=γ=90° One fourfold axis or one fourfold improper axis a=b≠cCubic α=β=γ=90° Four threefold axes at 109° 28′ to each other a=b=cdifferent space-filling patterns)! These are all documented in the International Tables forCrystallography (see Bibliography at end of the book). It is important not to lose sight of the fact that the lattice points represent equivalentpositions in a crystal structure and not atoms. In a real crystal, an atom, a complex ion, amolecule, or even a group of molecules could occupy a lattice point. The lattice pointsare used to simplify the repeating patterns within a structure, but they tell us nothing ofthe chemistry or bonding within the crystal—for that we have to include the atomicpositions: this we will do later in the chapter when we look at some real structures. It is instructive to note how much of a structure these various types of unit cellrepresent. We noted a difference between the centred and primitive two-dimensional unitcell where the centred cell contains two lattice points whereas the primitive cell containsonly one. We can work out similar occupancies for the three-dimensional case. Thenumber of unit cells sharing a particular molecule depends on its site. A corner site isshared by eight unit cells, an edge site by four, a face site by two and a molecule at thebody-centre is not shared by any other unit cell (Figure 1.25). Using these figures, we canwork out the number of molecules in each of the four types of cell in Figure 1.24,assuming that one molecule is occupying each lattice point. The results are listed in Table1.4.
An introduction to crystal structures 27 FIGURE 1.24 Primitive (a), body- centred (b), face-centred (c), and face- centred (A, B, or C) (d), unit cells, 1.5.5 MILLER INDICESThe faces of crystals, both when they grow and when they are formed by cleavage, tendto be parallel either to the sides of the unit cell or to planes in the crystal that contain ahigh density of atoms. It is useful to be able to refer to both crystal faces and to the planesin the crystal in some way—to give them a name—and this is usually done by usingMiller indices. First, we will describe how Miller indices are derived for lines in two-dimensionalnets, and then move on to look at planes in three-dimensional lattices. Figure 1.26 is arectangular net with several sets of lines, and a unit cell is marked on each set with theorigin of each in the bottom left-hand corner corresponding to the directions of the x and
Solid state chemistry 28y axes. A set of parallel lines is defined by two indices, h and k, where h and k are thenumber of parts into which a and b, the unit cell edges, are divided by the lines. Thus theindices of a line hk are defined so that the line intercepts a at and b at . Start byfinding a line next to the one passing through the origin, In the set of lines marked A, theline next to the one passing through the origin TABLE 1.3 Bravais latticesCrystal system Lattice typesCubic P, I, FTetragonal P, I
An introduction to crystal structures 29Orthorhombic P, C, I, FHexagonal PTrigonal (Rhombohedral) P/RaMonoclinic P, CTriclinic PaThe primitive description of the rhombohedral lattice is normally given the symbol R. TABLE 1.4 Number of molecules in four types of cellsName Symbol Number of molecules in unit cellPrimitive P 1Body-centred I 2Face-centred A or B or C 2All face-centred F 4leaves a undivided but divides b into two; both intercepts lie on the positive side of theorigin, therefore, in this case, the indices of the set of lines hk are 12 (referred to as the‘one-two’ set). If the set of lines lies parallel to one of the axes then there is no interceptand the index becomes zero. If the intercepted cell edge lies on the negative side of theorigin, then the index is written with a bar on the top (e.g., ), known as ‘bar-two’. Noticethat if we had selected the line on the other side of the origin in A we would have indexedthe lines as the no difference exists between the two pairs of indices and always thehk and the lines are the same set of lines. Try Question 5 for more examples. Noticealso, in Figure 1.26, that the lines with the lower indices are more widely spaced. The Miller indices for planes in three-dimensional lattices are given by hkl, where l isnow the index for the z-axis. The principles are the same. Thus a plane is indexed hklwhen it makes intercepts and with the unit cell edges a, b, and c. Figure 1.27depicts some cubic lattices with various planes shaded. The positive directions of the axesare marked, and these are orientated to conform to
Solid state chemistry 30FIGURE 1.25 Unit cells showing amolecule on (a) a face, (b) an edge,and (c) a corner.FIGURE 1.26 A rectangular netshowing five sets of lines, A–E, withunit cells marked.
An introduction to crystal structures 31the conventional right-hand rule as illustrated in Figure 1.28. In Figure 1.27(a), theshaded planes lie parallel to y and z, but leave the unit cell edge a undivided; the Millerindices of these planes are thus 100. Again, take note that the hkl and planes are thesame. 1.5.6 INTERPLANAR SPACINGSIt is sometimes useful to be able to calculate the perpendicular distance dhkl betweenparallel planes (Miller indices hkl). When the axes are at right angles to one another(orthogonal) the geometry is simple and for an orthorhombic system where a≠b ≠c andα=β=γ=90°, this gives:Other relationships are summarized in Table 1.5. 1.5.7 PACKING DIAGRAMSDrawing structures in three-dimensions is not easy and so crystal structures are oftenrepresented by two-dimensional plans or projections of the unit cell contents—in muchthe same way as an architect makes building plans. These projections are called packingdiagrams because they are particularly useful in molecular structures
Solid state chemistry 32FIGURE 1.27 (a)–(c) Planes in a face-centred cubic lattice, (d) Planes in abody-centred cubic lattice (two unitcells are shown).
An introduction to crystal structures 33 FIGURE 1.28 The right-handed rule for labelling axes.for showing how the molecules pack together in the crystal, and thus the intermolecularinteractions. The position of an atom or ion in a unit cell is described by its fractional coordinates;these are simply the coordinates based on the unit cell axes (known as thecrystallographic axes), but expressed as fractions of the unit cell lengths. It has thesimplicity of a universal system which enables unit cell positions to be compared fromstructure to structure regardless of variation in unit cell size. TABLE 1.5 d-spacings in different crystal systemsCrystal system dhkl, as a function of Miller indices and lattice parametersCubicTetragonalOrthorhombicHexagonal
Solid state chemistry 34Monoclinic FIGURE 1.29 Packing diagram for a body-centred unit cell.To take a simple example, in a cubic unit cell with a=1000 pm, an atom with an xcoordinate of 500 pm has a fractional coordinate in the x direction ofSimilarly, in the y and z directions, the fractional coordinates are given by andrespectively. A packing diagram is shown in Figure 1.29 for the body-centred unit cell of Figure1.8. The projection is shown on the yx plane (i.e., we are looking at the unit cell straightdown the z-axis). The z-fractional coordinate of any atoms/ions lying in the top or bottomface of the unit cell will be 0 or 1 (depending on where you take the origin) and it isconventional for this not to be marked on the diagram. Any z-coordinate that is not 0 or 1is marked on the diagram in a convenient place. There is an opportunity to practiceconstructing these types of diagram in the questions at the end of the chapter. 1.6 CRYSTALLINE SOLIDSWe start this section by looking at the structures of some simple ionic solids. Ions tend tobe formed by the elements in the Groups at the far left and far right of the Periodic Table.Thus, we expect the metals in Groups I and II to form cations and the nonmetals ofGroups VI(16) and VII(17) and nitrogen to form anions, because by doing so they areable to achieve a stable noble gas configuration. Cations can also be formed by some ofthe Group III(13) elements, such as aluminium, Al3+, by some of the low oxidation statetransition metals and even occasionally by the high atomic number elements in GroupIV(14), such as tin and lead, giving Sn4+ and Pb4+. Each successive ionization becomes
An introduction to crystal structures 35more difficult because the remaining electrons are more strongly bound due to the greatereffective nuclear charge, and so highly charged ions are rather rare. An ionic bond is formed between two oppositely charged ions because of theelectrostatic attraction between them. Ionic bonds are strong but are also non-directional;their strength decreases with increasing separation of the ions. Ionic crystals are thereforecomposed of infinite arrays of ions which have packed together in such a way as tomaximize the coulombic attraction between oppositely charged ions and to minimize therepulsions between ions of the same charge. We expect to find ionic compounds in thehalides and oxides of the Group I and II metals, and it is with these crystal structures thatthis section begins. However, just because it is possible to form a particular ion, does not mean that thision will always exist whatever the circumstances. In many structures, we find that thebonding is not purely ionic but possesses some degree of covalency: the electrons areshared between the two bonding atoms and not merely transferred from one to the other.This is particularly true for the elements in the centre of the Periodic Table. This point istaken up in Section 1.6.4 where we discuss the size of ions and the limitations of theconcept of ions as hard spheres. Two later sections (1.6.5 and 1.6.6) look at the crystalline structures of covalentlybonded species. First, extended covalent arrays are investigated, such as the structure ofdiamond—one of the forms of elemental carbon—where each atom forms strongcovalent bonds to the surrounding atoms, forming an infinite three-dimensional networkof localized bonds throughout the crystal. Second, we look at molecular crystals, whichare formed from small, individual, covalently-bonded molecules. These molecules areheld together in the crystal by weak forces known collectively as van der Waals forces.These forces arise due to interactions between dipole moments in the molecules.Molecules that possess a permanent dipole can interact with one another (dipole-dipoleinteraction) and with ions (charge-dipole interaction). Molecules that do not possess adipole also interact with each other because ‘transient dipoles’ arise due to the movementof electrons, and these in turn induce dipoles in adjacent molecules. The net result is aweak attractive force known as the London dispersion force, which falls off veryquickly with distance. Finally, in this section, we take a very brief look at the structures of some silicates—the compounds that largely form the earth’s crust. 1.6.1 IONIC SOLIDS WITH FORMULA MX The Caesium Chloride Structure (CsCl)A unit cell of the caesium chloride structure is shown in Figure 1.30. It shows a caesiumion, Cs+, at the centre of the cubic unit cell, surrounded by eight chloride
Solid state chemistry 36 FIGURE 1.30 The CsCl unit cell. Cs, blue sphere; Cl, grey spheres (or vice versa).ions, Cl−, at the corners. It could equally well have been drawn the other way round withchloride at the centre and caesium at the corners because the structure consists of twointerpenetrating primitive cubic arrays. Note the similarity of this unit cell to the body-centred cubic structure adopted by some of the elemental metals such as the Group I(alkali) metals. However, the caesium chloride structure is not body-centred cubicbecause the environment of the caesium at the centre of the cell is not the same as theenvironment of the chlorides at the corners: a body-centred cell would have chlorides atthe corners (i.e., at [0, 0, 0], etc. and at the body-centre ). Each caesium issurrounded by eight chlorines at the corners of a cube and vice versa, so the coordinationnumber of each type of atom is eight. The unit cell contains one formula unit of CsCl,with the eight corner chlorines each being shared by eight unit cells. With ionic structureslike this, individual molecules are not distinguishable because individual ions aresurrounded by ions of the opposite charge. Caesium is a large ion (ionic radii are discussed in detail later in Section 1.6.4) and sois able to coordinate eight chloride ions around it. Other compounds with large cationsthat can also accommodate eight anions and crystallize with this structure include CsBr,CsI, TlCl, TlBr, TlI, and NH4Cl. The Sodium Chloride (or Rock Salt) Structure (NaCl)Common salt, or sodium chloride, is also known as rock salt. It is mined all over theworld from underground deposits left by the dried-up remains of ancient seas, and hasbeen so highly prized in the past that its possession has been the cause of much conflict,most notably causing the ‘salt marches’ organized by Gandhi, and helping to spark offthe French Revolution. A unit cell of the sodium chloride structure is illustrated in Figure1.31. The unit cell is cubic and the structure consists of two interpenetrating face-centredarrays, one of Na+ and the other of Cl− ions. Each sodium ion is surrounded by sixequidistant chloride ions situated at the corners
An introduction to crystal structures 37 FIGURE 1.31 The NaCl unit cell. Na, blue spheres; Cl, grey spheres (or vice versa). FIGURE 1.32 The close-packed layers in NaCl. Na, blue spheres; Cl, grey spheres.of an octahedron and in the same way each chloride ion is surrounded by six sodium ions:we say that the coordination is 6:6. An alternative way of viewing this structure is to think of it as a cubic close-packedarray of chloride ions with sodium ions filling all the octahedral holes. The conventionalunit cell of a ccp array is an F face-centred cube (hence the cubic in ccp); the close-packed layers lie at right angles to a cube diagonal (Figure 1.32). Filling all the
Solid state chemistry 38octahedral holes gives a Na:Cl ratio of 1:1 with the structure as illustrated in Figure 1.31.Interpreting simple ionic structures in terms of the close-packing of one of the ions withthe other ion filling some or all of either the octahedral or tetrahedral holes, is extremelyuseful: it makes it particularly easy to see both the coordination geometry around aspecific ion and also the available spaces within a structure. As you might expect from their relative positions in Group I, a sodium ion is smallerthan a caesium ion and so it is now only possible to pack six chlorides around it and noteight as in caesium chloride. The sodium chloride unit cell contains four formula units of NaCl. If you find thisdifficult to see, work it out for yourself by counting the numbers of ions in the differentsites and applying the information given in Table 1.4. Table 1.6 lists some of the compounds that adopt the NaCl structure; more than 200are known. TABLE 1.6 Compounds that have the NaCl (rock-salt) type of crystal structureMost alkali halides, MX, and AgF, AgCl, AgBrAll the alkali hydrides, MHMonoxides, MO, of Mg, Ca, Sr, BaMonosulfides, MS, of Mg, Ca, Sr, Ba FIGURE 1.33 (a) An [MX6] octahedron, (b) a solid octahedron, and (c) plan of an octahedron with contours.Many of the structures described in this book can be viewed as linked octahedra, whereeach octahedron consists of a metal atom surrounded by six other atoms situated at thecorners of an octahedron (Figure 1.33(a) and Figure 1.33(b)). These can also be depicted
An introduction to crystal structures 39as viewed from above with contours marked, as in Figure 1.33(c). Octahedra can linktogether via corners, edges, and faces, as seen in Figure 1.34. The FIGURE 1.34 The conversion of (a) corner-shared MX6 octahedra to (b) edge-shared octahedra, and (c) edge- shared octahedra to (d) face-shared octahedra.
Solid state chemistry 40 FIGURE 1.35 NaCl structure showing edge-sharing of octahedra and the enclosed tetrahedral space (shaded).linking of octahedra by different methods effectively eliminates atoms because some ofthe atoms are now shared between them: two MO6 octahedra linked through a vertex hasthe formula, M2O11; two MO6 octahedra linked through an edge has the formula, M2O10;two MO6 octahedra linked through a face has the formula, M2O9. The NaCl structure can be described in terms of NaCl6 octahedra sharing edges. Anoctahedron has 12 edges, and each one is shared by two octahedra in the NaCl structure.This is illustrated in Figure 1.35, which shows a NaCl unit cell with three NaCl6octahedra shown in outline, and one of the resulting tetrahedral spaces is depicted byshading. The Nickel Arsenide Structure (NiAs)The nickel arsenide structure is the equivalent of the sodium chloride structure inhexagonal close-packing. It can be described as an hcp array of arsenic atoms with nickelatoms occupying the octahedral holes. The geometry about the nickel atoms is thusoctahedral. This is not the case for arsenic: each arsenic atom sits in the centre of atrigonal prism of six nickel atoms (Figure 1.36).
An introduction to crystal structures 41 The Zinc Blende (or Sphalerite) and Wurtzite Structures (ZnS)Unit cells of these two structures are shown in Figure 1.37 and Figure 1.38, respectively.They are named after two different naturally occurring mineral forms of zinc sulfide.Zinc blende is often contaminated by iron, making it very dark in colour and thus lendingit the name of ‘Black Jack’. Structures of the same element or compound that differ onlyin their atomic arrangements are termed polymorphs. FIGURE 1.36 (a) The unit cell of nickel arsenide, NiAs. (For undistorted hcp c/a=1.633, but this ratio is found to vary considerably.) Ni, blue spheres; As, grey spheres, (b) The trigonal prismatic coordination of arsenic in NiAs.
Solid state chemistry 42FIGURE 1.37 The crystal structure ofzinc blende or sphalerite, ZnS. Zn,blue spheres; S, grey spheres (or viceversa).FIGURE 1.38 The crystal structure ofwurtzite, ZnS. Zn, blue spheres; S,grey spheres.
An introduction to crystal structures 43The zinc blende structure can be described as a ccp array of sulfide ions with zinc ionsoccupying every other tetrahedral hole in an ordered manner. Each zinc ion is thustetrahedrally coordinated by four sulfides and vice versa. Compounds adopting thisstructure include the copper halides and Zn, Cd, and Hg sulfides. Notice that if all theatoms were identical, the structure would be the same as that of a diamond (see Section1.6.5). Notice that the atomic positions are equivalent, and we could equally wellgenerate the structure by swapping the zinc and sulfurs. The wurtzite structure is composed of an hcp array of sulfide ions with alternatetetrahedral holes occupied by zinc ions. Each zinc ion is tetrahedrally coordinated by foursulfide ions and vice versa. Compounds adopting the structure include BeO, ZnO, andNH4F. Notice how the coordination numbers of the structures we have observed so far havechanged. The coordination number for close-packing, where all the atoms are identical, istwelve. In the CsCl structure, it is eight; in NaCl, it is six; and in both of the ZnSstructures, it is four. Generally, the larger a cation is, the more anions it can pack arounditself (see Section 1.6.4). 1.6.2 SOLIDS WITH GENERAL FORMULA MX2 The Fluorite and Antifluorite StructuresThe fluorite structure is named after the mineral form of calcium fluoride, CaF2, which isfound in the U.K. in the famous Derbyshire ‘Blue John’ mines. The structure is illustratedin Figure 1.39. It can be described as related to a ccp array of calcium ions with fluoridesoccupying all of the tetrahedral holes. There is a problem with this as a descriptionbecause calcium ions are rather smaller than fluoride ions, and so, physically, fluorideions would not be able to fit into the tetrahedral holes of a calcium ion array.Nevertheless, it gives an exact description of the relative positions of the ions. Thediagram in Figure 1.39(a) depicts the fourfold tetrahedral coordination
Solid state chemistry 44FIGURE 1.39 The crystal structure offluorite, CaF2. (a) Computer generatedunit cell as a ccp array of cations: Ca,
An introduction to crystal structures 45 blue spheres; grey spheres, (b) and (c) The same structure redrawn as a primitive cubic array of anions. (d) Relationship of unit cell dimensions to the primitive anion cube (the octant).of the fluoride ions very clearly. Notice also that the larger octahedral holes are vacant inthis structure—one of them is located at the body-centre of the unit cell in Figure 1.39(a).This becomes a very important feature when we come to look at the movement of ionsthrough defect structures in Chapter 5. By drawing cubes with fluoride ions at each corner as has been done in Figure 1.39(b),you can see that there is an eightfold cubic coordination of each calcium cation. Indeed, itis possible to move the origin and redraw the unit cell so that this feature can be seenmore clearly as has been done in Figure 1.39(c). The unit cell is now divided into eightsmaller cubes called octants, with each alternate octant occupied by a calcium cation. In the antifluorite structure, the positions of the cations and anions are merelyreversed, and the description of the structure as cations occupying all the tetrahedral holesin a ccp array of anions becomes more realistic. In the example with the biggest anionand smallest cation, Li2Te, the telluriums are approximately close-packed (even thoughthere is a considerable amount of covalent bonding). For the other compounds adoptingthis structure, such as the oxides and sulfides of the alkali metals, M2O and M2S, thedescription accurately shows the relative positions of the atoms. However, the anionscould not be described as close-packed because they are not touching. The cations are toobig to fit in the tetrahedral holes, and, therefore, the anion-anion distance is greater thanfor close-packing. These are the only structures where 8:4 coordination is found. Many of the fast-ionconductors are based on these structures (see Chapter 5, Section 5.4). The Cadmium Chloride (CdCl2) and Cadmium Iodide (CdI2) StructuresBoth of these structures are based on the close-packing of the appropriate anion with halfof the octahedral holes occupied by cations. In both structures, the cations occupy all theoctahedral holes in every other anion layer, giving an overall layer structure with 6:3coordination. The cadmium chloride structure is based on a ccp array of chloride ionswhereas the cadmium iodide structure is based on an hcp array of iodide ions. Thecadmium iodide structure is shown in Figure 1.40, and in (a) we can see that an iodideanion is surrounded by three cadmium cations on one side but by three iodides on theother (i.e., it is not completely surrounded by ions of the opposite charge as we wouldexpect for an ionic structure). This is evidence that the bonding in some of thesestructures is not entirely ionic, as we have tended to imply so far. This point is discussedagain in more detail in Section 1.6.4.
Solid state chemistry 46 The Rutile StructureThe rutile structure is named after one mineral form of titanium oxide (TiO2). Rutile has avery high refractive index, scattering most of the visible light incident on it, and so is themost widely used white pigment in paints and plastics. A unit cell is illustrated in Figure1.41. The unit cell is tetragonal and the structure again demonstrates 6:3 FIGURE 1.40 (a) The crystal structure of cadmium iodide, CdI2; (b) the structure of the layers in CdI2 and CdCl2: the halogen atoms lie in planes above and below that of the metal
An introduction to crystal structures 47 atoms; and (c) the coordination around one iodine atom in CdI2. Cd, blue spheres; I, grey spheres.coordination but is not based on close-packing: each titanium atom is coordinated by sixoxygens at the corners of a (slightly distorted) octahedron and each oxygen atom issurrounded by three planar titaniums which lie at the corners of an (almost) equilateraltriangle. It is not geometrically possible for the coordination around Ti to be a perfectoctahedron and for the coordination around O to be a perfect equilateral triangle. The structure can be viewed as chains of linked TiO6 octahedra, where eachoctahedron shares a pair of opposite edges, and the chains are linked by sharing vertices:this is shown in Figure 1.41(b). Figure 1.41(c) shows a plan of the unit cell looking downthe chains of octahedra so that they are seen in projection. Occasionally the antirutile structure is encountered where the metal and non-metalshave changed places, such as in Ti2N.
Solid state chemistry 48FIGURE 1.41 The crystal structure ofrutile, TiO2. (a) Unit cell, (b) parts oftwo chains of linked [TiO6] octahedra,and (c) projection of structure on base
An introduction to crystal structures 49 of unit cell. Ti, blue spheres; O, grey spheres. The β-cristobalite StructureThe β-cristobalite structure is named after one mineral form of silicon dioxide, SiO2. Thesilicon atoms are in the same positions as both the zinc and sulfurs in zinc blende (or thecarbons in diamond, which we look at later in Section 1.6.5): each pair of silicon atoms isjoined by an oxygen midway between. The only metal halide adopting this structure isberyllium fluoride, BeF2, and it is characterized by 4:2 coordination. 1.6.3 OTHER IMPORTANT CRYSTAL STRUCTURESAs the valency of the metal increases, the bonding in these simple binary compoundsbecomes more covalent and the highly symmetrical structures characteristic of the simpleionic compounds occur far less frequently, with molecular and layer structures beingcommon. Many thousands of inorganic crystal structures exist. Here we describe just afew of those that are commonly encountered and those that occur in later chapters. The Bismuth Triiodide Structure (BiI3)This structure is based on an hcp array of iodides with the bismuths occupying one-thirdof the octahedral holes. Alternate pairs of layers have two-thirds of the octahedral sitesoccupied. Corundum α-Al2O3This mineral is the basis for ruby and sapphire gemstones, their colour depending on theimpurities. It is very hard—second only to diamond. This structure may be described asan hcp array of oxygen atoms with two-thirds of the octahedral holes occupied byaluminium atoms. As we have seen before, geometrical constraints dictate that octahedralcoordination of the aluminiums precludes tetrahedral coordination of the oxygens.However, it is suggested that this structure is adopted in preference to other possible onesbecause the four aluminiums surrounding an oxygen approximate most closely to aregular tetrahedron. The structure is also adopted by Ti2O3, V2O3, Cr2O3, α-Fe2O3, α-Ga2O3, and Rh2O3. The Rhenium Trioxide Structure (ReO3)This structure (also called the aluminium fluoride structure) is adopted by the fluorides ofAl, Sc, Fe, Co, Rh, and Pd; also by the oxides WO3 (at high temperature) and ReO3 (seeChapter 5, Section 5.8.1). The structure consists of ReO6 octahedra linked togetherthrough each corner to give a highly symmetrical three-dimensional network with cubicsymmetry. Part of the structure is given in Figure 1.42(a), the linking of the octahedra in(b), and the unit cell in (c).
Solid state chemistry 50. FIGURE 1.42 (a) Part of the ReO3 structure, (b) ReO3 structure showing the linking of [ReO6] octahedra, and
An introduction to crystal structures 51 (c) unit cell. Re, blue spheres; O, grey spheres. Mixed Oxide StructuresThree important mixed oxide structures exist: spinel, perovskite, and ilmeniteThe Spinel and Inverse-spinel StructuresThe spinels have the general formula AB2O4, taking their name from the mineral spinelMgAl2O4: generally, A is a divalent ion, A2+, and B is trivalent, B3+. The structure can bedescribed as being based on a cubic close-packed array of oxide ions, with A2+ ionsoccupying tetrahedral holes and B3+ ions occupying octahedral FIGURE 1.43 The spinel structure, CuAl2O4 (AB2O4). See colour insert following page 196. Cu, blue spheres; Al, pink spheres; O, red spheres.holes. A spinel crystal containing n AB2O4 formula units has 8n tetrahedral holes and 4noctahedral holes; accordingly, one-eighth of the tetrahedral holes are occupied by A2+ions and one-half of the octahedral holes by the B3+ ions. A unit cell is illustrated inFigure 1.43. The A ions occupy tetrahedral positions together with the corners and face-centres of the unit cell. The B ions occupy octahedral sites. Spinels with this structureinclude compounds of formula MAl2O4 where M is Mg, Fe, Co, Ni, Mn, or Zn. When compounds of general formula AB2O4 adopt the inverse-spinel structure, theformula is better written as B(AB)O4, because this indicates that half of the B3+ ions nowoccupy tetrahedral sites, and the remaining half, together with the A2+ ions, occupy the
Solid state chemistry 52octahedral sites. Examples of inverse-spinels include magnetite, Fe3O4, (see Chapter 9,Section 9.7) Fe(MgFe)O4, and Fe(ZnFe)O4.The Perovskite StructureThis structure is named after the mineral CaTiO3. A unit cell is shown in Figure 1.44(a):This unit cell is known as the A-type because if we take the general formula ABX3 forthe perovskites, then theA atom is at the centre in this cell. The central Ca (A) atom iscoordinated to 8 Ti atoms (B) at the corners and to 12 oxygens (X) at the midpoints of thecell edges. The structure can be usefully described in other ways. First, it can bedescribed as a ccp array of A and X atoms with the B atoms occupying the octahedralholes (compare with the unit cell of NaCl in Figure 1.31 if you want to check this).Second, perovskite has the same octahedral framework as ReO3 based on BX6 octahedrawith an A atom added in at the centre of the cell (Figure 1.42(b)). Compounds adoptingthis structure include SrTiO3, SrZrO3, SrHfO3, SrSnO3, and BaSnO3. The structures of thehigh temperature superconductors are based on this structure (see Chapter 10, Section10.3.1). FIGURE 1.44 The perovskite structure of compounds ABX3, such as CaTiO3. See colour insert following page 196. Ca, green sphere; Ti, silver spheres; O, red spheres.The Ilmenite StructureThe ilmenite structure is adopted by oxides of formula ABO3 when A and B are similar insize and their total charge adds up to +6. The structure is named after the mineral ofFeIITiIVO3, and the structure is very similar to the corundum structure described
An introduction to crystal structures 53previously, an hcp array of oxygens, but now two different cations are present occupyingtwo-thirds of the octahedral holes. The structures related to close-packing are summarized in Table 1.7. 1.6.4 IONIC RADIIWe know from quantum mechanics that atoms and ions do not have precisely definedradii. However, from the foregoing discussion of ionic crystal structures we have seenthat ions pack together in an extremely regular fashion in crystals, and their atomicpositions, and thus their interatomic distances, can be measured very accurately. It is avery useful concept, therefore, particularly for those structures based on close-packing, tothink of ions as hard spheres, each with a particular radius. If we take a series of alkali metal halides, all with the rock salt structure, as we replaceone metal ion with another, say sodium with potassium, we would expect the metal-halide internuclear distance to change by the same amount each time if the concept of anion as a hard sphere with a particular radius holds true. Table 1.8 presents the results ofthis procedure for a range of alkali halides, and the change in internuclear distance onswapping one ion for another is highlighted. From Table 1.8, we can see that the change in internuclear distance on changing theion is not constant, but also that the variation is not great: this provides us with someexperimental evidence that it is not unreasonable to think of the ions as having a fixedradius. We can see, however, that the picture is not precisely true, neither would weexpect it to be, because atoms and ions are squashable entities and their TABLE 1.7 Structures related to close-packed arrangements of anions ExamplesFormula Cation:anion Type and Cubic close-packing Hexagonal close- coordination number of holes packing occupiedMX 6:6 All octahedral Sodium chloride: Nickel arsenide: NaCl, FeO, MnS, NiAs, FeS, NiS TiC 4:4 Half tetrahedral; Zinc blende: ZnS, Wurtzite: ZnS, every alternate CuCl, γ-AgI β-AgI site occupiedMX2 8:4 All tetrahedral; Fluorite: CaF2, ThO2, None ZrO2, CeO2 6:3 Half octahedral; Cadmium chloride: Cadmium iodide: alternate layers CdCl2 CdI2, TiS2 have fully occupied sitesMX3 6:2 One-third Bismuth iodide: octahedral; BiI3, FeCl3, TiCl3,
Solid state chemistry 54 alternate pairs of VCl3 layers have two- thirds of the octahedral sites occupiedM2X3 6:4 Two-thirds Corundum: octahedral α-Al2O3, α-Fe2O3, V2O3, Ti2O3, α-Cr2O3ABO3 Two-thirds Ilmenite: FeTiO3 octahedralAB2O4 One-eighth Spinel: MgAl2O4 Olivine: Mg2SiO4 tetrahedral and inverse spinel: one-half MgFe2O4, Fe3O4 octahedralsize is going to be affected by their environment. Nevertheless, it is a useful concept todevelop a bit further as it enables us to describe some of the ionic crystal structures in asimple pictorial way. There have been many suggestions as to how individual ionic radii can be assigned,and the literature contains several different sets of values. Each set is named after theperson(s) who originated the method of determining the radii. We will describe some ofthese methods briefly before listing the values most commonly used at present. It is mostimportant to remember that you must not mix radii from more than one set of values.Even though the values vary considerably from set to set, each set is internally consistent(i.e., if you add together two radii from one set TABLE 1.8 Interatomic distances of some alkali halides, rM-x/pm F− Cl− Br− I−Li+ 201 56 257 18 275 27 302 30 24 23 21Na+ 231 50 281 17 298 25 323 35 33 31 30K+ 266 48 314 15 329 24 353 16 14 14 13Rb+ 282 46 328 15 343 23 366of values, you will obtain an approximately correct internuclear distance as determinedfrom the crystal structure). The internuclear distances can be determined by X-ray crystallography. In order toobtain values for individual ionic radii from these, the value of one radius needs to befixed by some method. Originally in 1920, Landé suggested that in the alkali halide with
An introduction to crystal structures 55the largest anion and smallest cation—LiI—the iodide ions must be in contact with eachother with the tiny Li+ ion inside the octahedral hole: as the Li-I distance is known, it isthen a matter of simple geometry to determine the iodide radius. Once the iodide radius isknown then the radii of the metal cations can be found from the structures of the metaliodides—and so on. Bragg and Goldschmidt later extended the list of ionic radii usingsimilar methods. It is very difficult to come up with a consistent set of values for the ionicradii, because of course the ions are not hard spheres, they are somewhat elastic, and theradii are affected by their environment such as the nature of the oppositely charged ligandand the coordination number. Pauling proposed a theoretical method of calculating theradii from the internuclear distances; he produced a set of values that is both internallyconsistent and shows the expected trends in the Periodic Table. Pauling’s method was totake a series of alkali halides with isoelectronic cations and anions and assume that theyare in contact: if you then assume that each radius is inversely proportional to theeffective nuclear charge felt by the outer electrons of the ion, a radius for each ion can becalculated from the internuclear distance. Divalent ions undergo additional compressionin a lattice and compensation has to be made for this effect in calculating their radii. Withsome refinements this method gave a consistent set of values that was widely used formany years; they are usually known as effective ionic radii. It is also possible to determine accurate electron density maps for the ionic crystalstructures using X-ray crystallography. Such a map is shown for NaCl and LiF in Figure1.45. The electron density contours fall to a minimum—although not to zero—in betweenthe nuclei and it is suggested that this minimum position should be taken as the radiusposition for each ion. These experimentally determined ionic radii are often calledcrystal radii; the values are somewhat different from the older sets and tend to make theanions smaller and the cations bigger than previously. The most comprehensive set ofradii has been compiled by FIGURE 1.45 Electron density maps for (a) NaCl and (b) LiF.